| ||Format||Pages||Price|| |
|5||$43.00||  ADD TO CART|
|Hardcopy (shipping and handling)||5||$43.00||  ADD TO CART|
Significance and Use
where L1 and L2 are the specimen lengths at temperatures T1 and T2, respectively. α is, therefore, obtained by dividing the linear expansion per unit length by the change in temperature.
5.2 The nature of most plastics and the construction of the dilatometer make −30 to +30°C (−22°F to +86°F) a convenient temperature range for linear thermal expansion measurements of plastics. This range covers the temperatures in which plastics are most commonly used. Where testing outside of this temperature range or when linear thermal expansion characteristics of a particular plastic are not known through this temperature range, particular attention shall be paid to the factors mentioned in 1.2 and special preliminary investigations by thermo-mechanical analysis, such as that prescribed in Practice D4065 for the location of transition temperatures, may be required to avoid excessive error. Other ways of locating phase changes or transition temperatures using the dilatometer itself may be employed to cover the range of temperatures in question by using smaller steps than 30°C (86°F) or by observing the rate of expansion during a steady rise in temperature of the specimen. Once such a transition point has been located, a separate coefficient of expansion for a temperature range below and above the transition point shall be determined. For specification and comparison purposes, the range from −30°C to +30°C (−22°F to +86°F) (provided it is known that no transition exists in this range) shall be used.
1.1 This test method covers determination of the coefficient of linear thermal expansion for plastic materials having coefficients of expansion greater than 1 × 10−6/°C by use of a vitreous silica dilatometer. At the test temperatures and under the stresses imposed, the plastic materials shall have a negligible creep or elastic strain rate or both, insofar as these properties would significantly affect the accuracy of the measurements.
1.1.1 Test Method E228 shall be used for temperatures other than −30°C to 30°C.
1.2 The thermal expansion of a plastic is composed of a reversible component on which are superimposed changes in length due to changes in moisture content, curing, loss of plasticizer or solvents, release of stresses, phase changes and other factors. This test method is intended for determining the coefficient of linear thermal expansion under the exclusion of these factors as far as possible. In general, it will not be possible to exclude the effect of these factors completely. For this reason, the test method can be expected to give only an approximation to the true thermal expansion.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D618 Practice for Conditioning Plastics for Testing
D883 Terminology Relating to Plastics
D4065 Practice for Plastics: Dynamic Mechanical Properties: Determination and Report of Procedures
E228 Test Method for Linear Thermal Expansion of Solid Materials With a Push-Rod Dilatometer
E691 Practice for Conducting an Interlaboratory Study to Determine the Precision of a Test Method
E831 Test Method for Linear Thermal Expansion of Solid Materials by Thermomechanical Analysis
ICS Number Code 83.080.01 (Plastics in general)
UNSPSC Code 13100000(Rubber and elastomers)
ASTM D696-08e1, Standard Test Method for Coefficient of Linear Thermal Expansion of Plastics Between −30°C and 30°C with a Vitreous Silica Dilatometer, ASTM International, West Conshohocken, PA, 2008, www.astm.orgBack to Top